Research article ISSN 2234-7658 (print) / ISSN 2234-7666 (online) http://dx.doi.org/10.5395/rde.2014.39.1.32
Antibacterial effect of self-etching adhesive systems on Streptococcus mutans Seung-Ryong Kim, Dong-Hoon Shin* Department of Conservative Dentistry, Dankook University College of Dentistry and Institute of Dental Science, Cheonan, Korea
Objectives: In this study, we evaluated the antibacterial activity of self-etching adhesive systems against Streptococcus mutans using the agar diffusion method. Materials and Methods: Three 2-step systems, Clearfil SE Bond (SE, Kuraray), Contax (CT, DMG), and Unifil Bond (UnB, GC), and three 1-step systems, Easy Bond (EB, 3M ESPE), U-Bond (UB, Vericom), and All Bond SE (AB, BISCO) were used. 0.12% chlorhexidine (CHX, Bukwang) and 37% phosphoric acid gel (PA, Vericom) were used as positive controls. Results: The antibacterial activity of CHX and PA was stronger than that of the other groups, except SE. After light activation, the inhibition zone was reduced in the case of all 2-step systems except CT. However, all 1-step systems did not exhibit any inhibition zone upon the light activation. Conclusions: SE may be better than CT or UnB among the 2-step systems with respect to antibacterial activity, however, 1-step systems do not exhibit any antibacterial activity after light curing. (Restor Dent Endod 2014;39(1):32-38) Key words: Agar diffusion method; Antibacterial activity; Self-etching adhesive systems; S. mutans
Introduction Received October 31, 2013; Accepted December 10, 2013. Kim SR; Shin DH, Department of Conservative Dentistry, Dankook University College of Dentistry and Institute of Dental Science, Cheonan, Korea *Correspondence to Dong-Hoon Shin, DDS, PhD. Professor, Department of Conservative Dentistry, Dankook University College of Dentistry and Institute of Dental Science, San 7-1, Shinbu-dong, Dongnam-gu, Cheonan, Korea 330-716 TEL, +82-41-550-1965; FAX, +8241-553-1258; E-mail, [email protected]
Although the etiological factors of dental caries and the methods for its prevention have been widely investigated, secondary caries is still the main cause for the replacement of restorations.1 Several investigations have revealed microgaps at the interface between dentin and adhesive restorations in vivo.2,3 This implies that even the latest adhesive systems are not capable of producing a complete seal in clinical situations. Once the gaps are formed, bacteria and their toxic products readily invade. The bacteria proliferate at the bonding interface, permeate the unsealed dentinal tubules, and may cause pulpal responses. Therefore, the possibility of adhesive systems having antibacterial effects is attractive with respect to the prevention of infections. Elimination of bacteria during cavity preparation is another issue. Because it appears that only soft, wet dentin is heavily infected with bacteria, any techniques that effectively remove such infected dentin should be adequate to halt the carious process, if the cavity is then adequately sealed.4 In contrast, the removal of hard dry dentin, which is essentially only demineralized with relatively few bacteria present, would be unnecessary, and may result in the additional, unwarranted removal of a sound tooth structure and possible pulp exposure.5 Thus, after the removal of carious dentin, it is important to eliminate any remaining bacteria that may be present on the cavity
This is an Open Access article distributed under the terms of the Creative Commons Attribution Non-Commercial License (http://creativecommons.org/licenses/ by-nc/3.0) which permits unrestricted non-commercial use, distribution, and reproduction in any medium, provided the original work is properly cited.
©Copyrights 2014. The Korean Academy of Conservative Dentistry.
Antibacterial effect of self-etching adhesive systems
walls, in the smear layer, at the dentinoenamel junction, or in the dentinal tubules.6 During the removal of carious tissue, bacteria invariably remain entrapped in the dentinal substrate because neither the clinical parameters of dentin hardness and color nor the caries-detector dyes are able to ensure the complete elimination of microorganisms.5,7 Bonding systems that have intrinsic antibacterial properties would be beneficial in this regard. As the contemporary dentin adhesive systems have not been proven to be completely effective in eliminating the microleakage at the tooth/restoration interface, the incorporation of antibacterial agents into the adhesive materials has been proposed to prevent caries recurrence.8,9 An acid agent could have an antibacterial effect because of its low pH. Settembrini et al. reported that etchants removed the bacteria on cavity walls.10 However, selfetching adhesive systems do not use acid etching systems. Consequently, a cavity only needs to be air blown and not rinsed with water when these systems are used. That will save clinical chair time but may increase the chances of the survival of the bacteria remaining in the smear layer. An antibacterial effect is desired for restorative composites and adhesive systems in order to avoid the growth of the remaining bacteria in the cavity. This effect can be achieved by the incorporation of antibacterial agents, such as glutaraldehydes, fluorides, or antibacterial monomers in the formulation of adhesive systems. 11-16 In general, adhesive monomers of self-etching adhesive systems present a hydrophilic group at one end of the molecule, which is usually an acid, such as hydrogen phosphate or carboxylate. These traits provide these materials with a low pH and possibly some antibacterial properties. Therefore, not only antibacterial agents but also other substances commonly found in the adhesive system formulas, such as adhesion-promoting monomers that are acidic to different degrees, might exhibit some activity against bacterial growth.17,18 The components of a dentin bonding system are resinbased, like composite resin. It was found that a cured composite did not release any antibacterial components, producing no inhibition halo.17 Therefore, no elution of adequate amounts of antibacterial components from cured composites has been demonstrated. These results are not surprising since the fundamental components of composites exhibit little or no bacteriostatic/bactericidal effects against oral bacteria at low concentrations. Among the antibacterial agents incorporated into adhesive materials, the resin monomer 12-methacryloyloxy dodecyl-pyridinium bromide, known as MDPB, stands out.8,9,11,12 The main advantage of MDPB is its capacity to copolymerize with other resin monomers that are immobilized within the polymer matrix, which confers safety and prolonged antibacterial action to this agent. Furthermore, it does not leach to the medium. This
characteristic also ensures a good survival rate for the restoration, as MDPB, unlike soluble antibacterial agents, is not deleterious to the physical and mechanical properties of the adhesive materials.8,9 Although several studies describe the antibacterial effects of the MDPB monomer, little is known about the antibacterial effects of other self-etching adhesive systems. As the antibacterial effect occurs, other commercially available self-etching adhesive systems could also exhibit this antibacterial effect. This study was conducted to evaluate the antibacterial activity of 2-step and 1-step self-etching systems, with or without light activation, against Streptococcus mutans (S. mutans) by using an agar diffusion test (ADT). The null hypotheses were as follows: 1) There is no difference among inhibition zones, 2) light activation and pH do not influence the inhibition zone, irrespective of the bonding system.
Materials and methods Bacterial strain and culture S. mutans ATCC 25175 was used in this study. The bacteria were cultured in a tryptic soy broth (Difco Laboratories, Detroit, MI, USA) at 37℃ aerobically. The culture was started from freeze-dried stocks in 10 mL of a sterile tryptic soy broth. The culture was grown at 37℃ in an incubator (Hi-Tec Model 1S-61, Yamato Scientific Co. Ltd., Tokyo, Japan) for 24 hours. Preparation of specimens Three 2-step self-etching systems, Clearfil SE Bond (SE, Kuraray, Okayama, Japan), Contax (CT, DMG, Hamburg, Germany), and Unifil Bond (UnB, GC, Tokyo, Japan), and three 1-step self-etching systems, Easy Bond (EB, 3M ESPE, Saint Paul, MN, USA), U-Bond (UB, Vericom, Anyang, Korea), and All Bond SE (AB, BISCO, Schaumburg, IL, USA) were used for evaluating the antibacterial activity (Table 1). 0.12% chlorhexidine (CHX, Bukwang, Seoul, Korea) and 37% phosphoric acid (PA, Vericom) gel were used as the positive controls. 20 μL of each primer or bonding agent was applied to sterilized paper disks (diameter, 8 mm; thickness, 1.5 mm) with a pipette. A total of 10 specimens were used per group except for the positive and negative controls. Because the number of experimental and control groups was 20 (CHX, PA, three 2-step self-etching systems and three 1-step self-etching systems with or without light activation), the specimens were distributed into four petri dishes. Five paper disks smeared with the selfetching systems, CHX, and PA were placed on each petri dish. Another 20 μL of adhesives were applied and light activated in the case of the 2-step self-etching systems.
Kim SR and Shin DH Table 1. Specifications, main components, and manufacturers of the tested materials Adhesive system
Primer: HEMA, MDP, hydrophilic dimethacrylate, N,N-diethanol-p-toluidine, Clearfil SE Bond Two bottle Primer: 1.9 - 2 CQ, water. (SE, Kuraray, Japan) Two step Adhesive: 2.8 Adhesive: HEMA, MDP, hydrophobic dimethacrylate, N,N-diethanol-p-toluidine, CQ, silanized colloidal silica, BisGMA Unifil Bond (UnB, GC, Japan)
Two bottle Two step
Contax Two bottle (CT, DMG, Germany) Two step Adper Easy Bond (EB, 3M ESPE, USA)
One bottle One step
U-Bond One bottle (UB, VERICOM, Korea) One step All Bond SE (AB, BISCO, USA)
Two bottle One step
Primer: ethanol, HEMA, 4-META Adhesive : UDMA, HEMA
Primer: 3 Aqueous preparation of acrylic resin. Contains aromatic dimethacrylate, Adhesive: 5 polyol - mono-, dimethacrylate, polycarboxylicpolymethacrylate. 2.7 1-2 2.2
Methacrylated phosphoric esters, Vitrebon Copolymer, nanofiller, ethanol, water, dimethacrylates, HEMA, initiators Acetone, water, fumed silica, UDMA, 4-META, additives PART I: ethanol, sodium benzene sulfinate PART II: hydroxyethyl methacrylate, bis(glyceryl 1,3 dimethyacrylate) phosphate, biphenyl dimethacrylate
MDP, Methacryloyloxy decyl dihydrogenphosphate; CQ, Camphorquinone; UDMA, Urethane dimethacrylate; HEMA, 2-Hydroxyethyl methacrylate; 4-META, 4-methacryloxy ethyl trimellitate anhydride.
Figure 1. Inhibition zone of self-etching systems. CHX, Chlorhexidine; PA, Phosphoric acid; SE, Clearfil SE Bond; UnB, Unifil Bond; CT, Contax; AB, All Bond SE; EB, Easy Bond; UB, U-Bond. Plate 1-1, 3-1, No light activation; Plate 2-1, 4-1, Light activation. Agar diffusion test The antibacterial activity of each bonding system was evaluated against the S. mutans ATCC 25175. From the culture, bacterial suspensions were prepared in a tryptic soy broth until a turbidity compatible with 0.5 MacFarland was obtained. This scale allowed the bacterial concentration of a suspension to be estimated by its turbidity, 0.5
corresponded to a concentration of 1.5 × 108 (CFU/mL) at an optical density of 550 nm. The specimen disks were placed on tryptic soy agar (Difco Laboratories) plates inoculated with S. mutans. The positive controls of 0.12% CHX and 37% PA gel were added onto the paper disks. The diameter of the inhibition zone produced around each disk was measured after 48 hours of incubation (Figure 1).
Antibacterial effect of self-etching adhesive systems Table 2. Width of the inhibition zones (mm) according to the material and light-activation condition Inhibition zones [Mean ± SD] Number of Material Results of two-way ANOVA Without light With light specimen activation activation 28.43 ± 0.59a CHX 40 Control 27.27 ± 1.11ab PA 40 Main effect 2-step self-etching system 1-step self-etching system
SE UnB CT AB EB UB
10 10 10 10 10 10
26.66 ± 0.27b 21.61 ± 0.35d 10.58 ± 0.35f 0g 10.87 ± 1.07f 18.65 ± 0.40e
24.81 ± 2.22c 17.41 ± 0.26e 10.76 ± 0.48f 0g 0g 0g
Bonding system Light activation
p < 0.001 p < 0.001
Interaction effect Bonding system x Light activation p < 0.001
Different letters indicate the statistically significant difference at p < 0.05. CHX, Chlorhexidine; PA, Phosphoric acid; SE, Clearfil SE Bond; UnB, Unifil Bond; CT, Contax; AB, All Bond SE; EB, Easy Bond; UB, U-Bond.
Statistical analysis The data were analyzed by using a two-way ANOVA (bonding agent and light activation) and a Scheffe test. A value of p < 0.05 was considered to be a significant difference.
Results The mean diameters and the standard deviation values of the antibacterial inhibition zones are given in Table 2. Control groups of CHX and PA exhibited the widest zone, 28.43 ± 0.59 mm and 27.27 ± 1.11 mm each. The inhibition zones of 2-step self-etching systems SE, UnB, and CT were 26.66 ± 0.27 mm, 21.61 ± 0.35 mm, and 10.58 ± 0.35 mm, respectively, when they were applied without light activation, while their zones became narrow in the order of SE (24.81 ± 2.22 mm), UnB (17.41 ± 0.26 mm), and CT (10.76 ± 0.48 mm). The inhibition zones of 1-step self-etching systems EB and UB were 10.87 ± 1.07 mm and 18.65 ± 0.49 mm, respectively, when they were uncured. However, these zones could not be formed when they were cured. The other 1-step self-etching system AB did not form any inhibition zone, irrespective of the light activation. Two-way ANOVA indicated significant differences for the ‘materials’ (p = 0.000) and ‘light activation’ (p = 0.000) factors and for the interaction between the factors (p = 0.000) (Table 2). The positive CHX control group exhibited the most effective antibacterial activity against S. mutans, and the PA group was the next. Among the experimental groups, SE was the most effective, and its inhibition zone did not differ from that of the 37% PA positive group
(Figure 1). All 2-step self-etching systems showed various inhibition zones with and without light activation. Light activation diminished the inhibition zone except in the case of CT. In contrast, all 1-step self-etching systems did not exhibit any antibacterial activity after light activation on the adhesive. EB and UB showed an inhibition zone when the agent remained in situ without light activation. However, the antibacterial effect vanished upon light activation. No inhibition zone was detected in the case of AB both with and without the light activation.
Discussion ADT was used because it is a widely employed methodology for the determination of the inhibitory activity of liquid substances, in addition to being a simple and easy-tohandle technique and facilitating the comparison to other studies.19 The advantage of this method is that it allows direct comparisons of test materials against the test microorganisms, indicating which test materials have the potential to eliminate bacteria in the local microenvironment. Further, the results of ADT can indicate the existence of diffusible components into an aqueous milieu. However, ADT has limitations in that it measures only the water-soluble components and the solubility and the diffusability of the test agent affect the inhibition zone.20 The results of this method do not depend only on the toxicity of the material for a particular microorganism but are also highly influenced by the diffusability of the material across the medium. A material that diffuses more easily will probably provide larger zones of microbial growth inhibition.21,22 Other variables such as inoculum
Kim SR and Shin DH
size, incubation time, and the material/agar contact may also affect the results. S. mutans colonization on tooth surfaces has been recognized in the etiology and pathogenesis of human dental caries.23 The ability of S. mutans to produce acid by sugar fermentation and its capacity for acid tolerance comprise key virulence factors involved in the development of dental caries.24 Acid production by S. mutans leads to low pH values in dental plaque and contributes to the demineralization of tooth enamel and initiation of caries formation.25 Accompanying the acidogenicity of S. mutans is its acid-tolerance or aciduricity. S. mutans maintains glycolytic capabilities even at pH 4.4, the level that is growth-inhibitory.26 S. mutans resists environmental acid stress by increasing the proton translocating F-ATPase activity in response to a low pH.27 This mechanism makes the intracellular pH more alkaline than the extracellular environment pH, which plays a critical role in the pathogenesis of dental caries.28 There are several studies that describe the bonding system incorporating antibacterial components. Bapna et al. studied the antibacterial activity of the Scotchbond adhesive resin to which various chemical agents were added. 29 Although their study was not oriented to develop an antibacterial bonding system, cured resins containing sodium ﬂuoride, dodecylamine, or bipyridine inhibited the growth and attachment of S. mutans. Kudou et al. attempted the incorporation of vancomycin or metronidazol to a 4-META/MMA-TBB resin in order to develop an antibacterial bonding system for direct pulp capping.30 They reported that the resin containing 1 - 5% vancomycin produced inhibition against all streptococci and actinomycetes tested, and the resin with vancomycin did not affect the tensile bond strength. Imazato et al. investigated the utilization of 5% MDPB with the self-etching adhesive system (Clearfil Protect Bond) against S. mutans, Lactobacillus casei, and Actinomyces naeslundii. 12 As unpolymerized MDPB exhibits strong bactericidal activity, the residual bacteria in the cavity can be inactivated when a MDPB-containing bonding system is applied. Further, the bacteria can be inhibited by the immobilized agent after light activation as in the case of the surface of MDPB-added composites. Therefore, by the incorporation of MDPB, a bonding system with antibacterial effects before and after setting can be achieved. The current findings demonstrate the different inhibition levels produced by different 2-step self-etching systems or 1-step self-etching systems. As speculated earlier, the main reasons for the inhibition of bacterial growth are probably the cytotoxicity of the monomer or the acidic pH of the self-etching primer.13 However, Imazato and Feuerstein et al. suggested that the benefit of a low pH environment exhibited by dentin bonding systems should be considered to be ‘limited’.17,31
It was presumed that a relatively low pH affected the inhibition zone. However, this no longer seems to be an important influential factor because of the small pH difference among systems considered in this study. In spite of the acidic nature of self-etching adhesive systems, this characteristic does not seem to be sufficient to completely eliminate the residual bacteria from dentin because this tissue acts as a solid buffering medium to acidic monomers.32 2-methacryloyloxy ethyl phenyl hydrogen phosphate (Phenyl-P), 4-methacryloyloxyethyl trimellitate anhydride (4-META), and 10-methacryloyloxydecyl dihydrogen phosphate (MDP) are the main acidic monomers contained in the formulation of self-etching adhesive systems and are capable of demineralizing and inﬁltrating the dentin substrate simultaneously. According to Ohmori et al., MDP has a higher inhibitory function against microorganisms than Phenyl-P.18 MDP is present in both the primer and the adhesive components of SE, which exhibited the best results among the experimental groups in this study. The inhibition of caries associated with bacteria was observed when the uncured specimens were tested, but the antibacterial effects were adversely affected by the curing. The polymerization of adhesive materials causes entrapment in the polymeric matrix and decreases the release of polymerizable antibacterial components, as well as adhesion-promoting acidic monomers.33 Nevertheless, even in the case of light activation, there was some antibacterial activity when the 2-step self-etching systems were applied to the paper disks. The formation of the zones of microbial growth inhibition when the adhesive systems were light-activated may be explained by the fact that a complete conversion of monomers into polymers does not occur and hence, residual monomers can be released to the medium.34 Furthermore, light is not capable of passing through a paper disk that is adequately impregnated with the adhesive components.33 The antibacterial effect might also be due to the release of the residual monomers present in the oxygen-inhibited layer.35 The methodology employed in the present study has some limitations with respect to the reproduction of the physiological conditions of the pulpo-dentinal complex, such as the presence of intratubular fluid and intra-pulpal pressure. Due to these limitations, the results obtained in in vitro studies cannot be directly extrapolated to an in vivo situation because they may not reﬂect the actual effect of the material when applied under clinical conditions. However, laboratory tests are indispensable because they are at the base of the scientific evidence pyramid providing research-based support and serving as a reference for clinical investigations. Therefore, although the present study demonstrated in vitro the antibacterial characteristics of some self-etching systems with and without light activation, further clinical trials should be conducted to determine the inhibitory effect of bonding systems against
Antibacterial effect of self-etching adhesive systems
cariogenic microorganisms. Moreover, other methods, such as the direct contact test and aging test, should be considered to compensate for the drawbacks of ADT.
Conclusions In this study, we found that the antibacterial activity of CHX and PA was higher than that of the other experimental groups, except the SE primer. Among the self-etching systems considered, SE exhibited the most effective antibacterial activity against S. mutans. After light activation, the inhibition zone was reduced in the case of all 2-step self-etching systems except CT. 1-step selfetching systems, such as AB, EB, and UB, did not exhibit the formation of any inhibition zone upon light activation.
Acknowledgement The present research was conducted by the research fund of Dankook University in 2012. Conflict of Interest: No potential conflict of interest relevant to this article was reported.
References 1. Palotie U, Vehkalahti MM. Reasons for replacement of restorations: dentists’ perceptions. Act Odontol Scand 2012;70:485-490. 2. Hahn P, Weyen G, Fischer P, Plogmann S, Hannig M. Marginal and internal adaptation of composite restorations to dentin in vivo and in vitro. Am J Dent 2008;21:356-360. 3. Lee MA, Seo DK, Son HH, Cho BH. Influence of rebonding procedures on microleakage of composite resin restorations. J Korean Acad Conserv Dent 2010;35: 164-172. 4. Kidd EA, Joyston-Bechal S, Beighton D. Microbiological validation of assessments of caries activity during cavity preparation. Caries Res 1993;27:402-408. 5. Yip HK, Stevenson AG, Beeley JA. The specificity of caries detector dyes in cavity preparation. Br Dent J 1994;176:417-421. 6. Brännström M, Nordenvall KJ. Bacterial penetration, pulpal reaction and the inner surface of Concise enamel bond. Composite fillings in etched and unetched cavities. J Dent Res 1978;57:3-10. 7. Ricketts DN, Kidd EA, Beighton D. Operative and microbiological validation of visual, radiographic and electronic diagnosis of occlusal caries in non-cavitated teeth judged to be in need of operative care. Br Dent J 1995;179:214-220. 8. Kim JS, Shin DH. Inhibitory effect on Streptococcus
mutans and mechanical properties of the chitosan containing composite resin. Restor Dent Endod 2013;38: 36-42. 9. Imazato S, Kinomoto Y, Tarumi H, Torii M, Russell RR, McCabe JF. Incorporation of antibacterial monomer MDPB into dentin primer. J Dent Res 1997;76:768-772. 10. Settembrini L, Boylan R, Strassler H, Scherer W. A comparison of antimicrobial activity of etchants used for a total etch technique. Oper Dent 1997;22:84-88. 11. Imazato S, Torii Y, Takatsuka T, Inoue K, Ebi N, Ebisu S. Bactericidal effect of dentin primer containing antibacterial monomer methacryloyloxydodecylpyridini um bromide (MDPB) against bacteria in human carious dentin. J Oral Rehabil 2001;28:314-319. 12. Imazato S, Kuramoto A, Takahashi Y, Ebisu S, Peters MC. In vitro antibacterial effects of the dentin primer of Clearfil Protect Bond. Dent Mater 2006;22:527-532. 13. Karanika-Kouma A, Dionysopoulos P, Koliniotou-Koubia E, Kolokotronis A. Antibacterial properties of dentin bonding systems, polyacid-modified composite resins and composite resins. J Oral Rehabil 2001;28:157-160. 14. Peris AR, Mitsui FH, Lobo MM, Bedran-russo AK, Marchi GM. Adhesive systems and secondary caries formation: assessment of dentin bond strength, caries lesions depth and fluoride release. Dent Mater 2007;23:308316. 15. Kim S, Song M, Roh BD, Park SH, Park JW. Inhibition of Streptococcus mutans biofilm formation on composite resins containing ursolic acid. Restor Dent Endod 2013; 38:65-72. 16. Walter R, Duarte WR, Pereira PN, Heymann HO, Swift EJ Jr, Arnold RR. In vitro inhibition of bacterial growth using different dental adhesive systems. Oper Dent 2007;32:388-393. 17. Imazato S. Antibacterial properties of resin composites and dentin bonding systems. Dent Mater 2003;19:449457. 18. Ohmori K, Maeda N, Kohno A. Evaluation of antibacterial activity of three dentin primers using an in vitro tooth model. Oper Dent 1999;24:279-285. 19. Gondim JO, Duque C, Hebling J, Giro EM. Influence of human dentine on the antibacterial activity of selfetching adhesive systems against cariogenic bacteria. J Dent 2008;36:241-248. 20. Tobias RS. Antibacterial properties of dental restorative materials: a review. Int Endod J 1988;21:155-160. 21. Abdulkader A, Duguid R, Saunders EM. The antimicrobial activity of endodontic sealers to anaerobic bacteria. Int Endod J 1996;29:280-283. 22. Siqueira JF Jr, Favieri A, Gahyva SM, Moraes SR, Lima KC, Lopes HP. Antimicrobial activity and flow rate of newer and established root canal sealers. J Endod 2000; 26:274-277. 23. Loesche WJ. Role of Streptococcus mutans in human
Kim SR and Shin DH
dental decay. Microbiol Rev 1986;50:353-380. 24. Hamada S, Koga T, Ooshima T. Virulence factors of Streptococcus mutans and dental caries prevention. J Dent Res 1984;63:407-411. 25. Fitzgerald RJ, Keyes PH. Demonstration of the etiologic role of streptococci in experimental caries in the hamster. J Am Dent Assoc 1960;61:9-19. 26. Bender GR, Thibodeau EA, Marquis RE. Reduction of acidurance of streptococcal growth and glycolysis by ﬂuoride and gramicidin. J Dent Res 1985;64:90-95. 27. Lemos JA, Burne RA. A model of efﬁciency: stress tolerance by Streptococcus mutans. Microbiology 2008; 154:3247-3255. 28. Banas JA. Virulence properties of Streptococcus mutans. Front Biosci 2004;9:1267-1277. 29. Bapna MS, Mukherjee S, Murphy R. The antimicrobial effect of an iron-binding agent on Streptococcus mutans. J Oral Rehabil 1992;19:111-113. 30. Kudou Y, Obara K, Kawashima T, Kubota M, Abe S, Endo T, Komatsu M, Okuda R. Addition of antibacterial agents
to MMA-TBB dentin bonding systems-inﬂuences on tensile bond strength and antibacterial effect. Dent Mater J 2000;19:65-74. 31. Feuerstein O, Matalon S, Slutzky H, Weiss EI. Antibacterial properties of self-etching dental adhesive systems. J Am Dent Assoc 2007;138:349-354. 32. Schmalz G, Ergücü Z, Hiller KA. Effect of dentin on the antibacterial activity of dentin bonding agents. J Endod 2004;30:352-358. 33. Imazato S, Kuramoto A, Kaneko T, Ebisu S, Russell RR. Comparison of antibacterial activity of simpliﬁed adhesive systems. Am J Dent 2002;15:356-360. 34. Cadenaro M, Antoniolli F, Sauro S, Tay FR, Di Lenarda R, Prati C, Biasotto M, Contardo L, Breschi L. Degree of conversion and permeability of dental adhesives. Eur J Oral Sci 2005;113:525-530. 35. Finger WJ, Lee KS, Podszun W. Monomers with low oxygen inhibition as enamel/dentin adhesives. Dent Mater 1996;12:256-261.